ARTICLE IN PRESS Journal of Magnetism and Magnetic Materials 321 (2009) 1389–1392
Contents lists available at ScienceDirect
Journal of Magnetism and Magnetic Materials journal homepage: www.elsevier.com/locate/jmmm
Preparation of NiZn-ferrite nanoﬁbers by electrospinning for DNA separation Joong-Hee Nam a,, Yong-Hui Joo a, Ji-Ho Lee b, Jeong Ho Chang b, Jeong Ho Cho a, Myoung Pyo Chun a, Byung Ik Kim a a b
Advanced Materials & Components Laboratory, Korea Institute of Ceramic Engineering and Technology, 233-5, Gasan-dong, Geumcheon-gu, Seoul 153-801, Republic of Korea Eco-Biomaterials Laboratory, Korea Institute of Ceramic Engineering and Technology, Seoul 153-801, Republic of Korea
a r t i c l e in fo
Available online 20 February 2009
We present the synthesis, magnetic and UV spectrometry of NiZn-ferrite nanoﬁber. The single phase of spinel ferrite was obtained at 600 1C. The NiZn-ferrite ﬁbers fabricated by an electrospinning process were formed as a polygonal grain growth with ﬁring temperature in ﬁber matrix. It appeared that the saturation magnetization (MS) of NiZn-ferrite nanoﬁber was dependent on Ni/Zn molar ratio which is similar to that of the inverse spinel ferrites. The NiZn-ferrite ﬁbers showed good DNA adsorption efﬁciency that can be modiﬁed and utilized for DNA separation with magnetic nanoﬁber as a novel material in clinical applications. & 2009 Elsevier B.V. All rights reserved.
Keywords: Ceramic nanoﬁber Electrospinning NiZn ferrite DNA separation
Although electrospinning techniques have been generally used for the fabrication of polymer nanoﬁbers, they are now also used for the preparation of ceramic nanoﬁbers including composite materials [1–7]. The possibility of extending this process to ceramic materials has started in nanostructure research for new applications. One reason for this increasing interest in electrospinning stems from the fact that it is a relatively inexpensive technique to make nanoﬁbers. With the expansion of electrospinning from polymers to composites and to ceramics, applications expand to the preparation of nanostructured materials. Their typical properties of having a high surface-to-volume ratio make them useful for potential applications such as nanoelectronic devices, sensors, solar cells, photonics, and multiferroic materials , molecular sieves , high-temperature insulation , catalysis , biomedical separation, and microwave absorbers. Recently, a few popular processes to produce ceramic nanoﬁber and inorganic-polymer composite ﬁber as well as polymer ﬁber have been reported . In general, ceramic nanoﬁbers are prepared by the electrospinning of ceramic precursors in the presence of polymers followed by calcination. Careful preparation of the precursors is essential to electrospun ceramic systems. Several parameters such as solvent volatility, viscosity, surface tension, conductivity, and applied voltage need to be controlled. Electrospinning methods usually adopt the cone-jet principle to manufacture ultra-thin ﬁbers. For this purpose, the electrospinning solution must have a high polymer concentration, high enough to cause entanglement with low viscosity to allow motion induced by the electric ﬁeld. To prevent the solvent from
Corresponding author. Tel.: +82 2 3282 2443; fax: +82 2 3282 7759.
E-mail address: [email protected]
(J.-H. Nam). 0304-8853/$ - see front matter & 2009 Elsevier B.V. All rights reserved. doi:10.1016/j.jmmm.2009.02.044
collapsing into droplets before it evaporates, the surface tension of the solution must be low. Morphological change of electrospun ﬁbers before calcinating can be strongly dependent upon the distance between nozzle needle and collector in various applied electrical ﬁeld, ﬂow rate, and ambient environment like temperature and humidity. The increase of needle-to-collector distance or decrease in the electrical ﬁeld may result in reduced bead density, regardless of the polymer solution concentration . The chemical synthesis of spinel ferrite-based particulates may represent an important step towards the engineering of typical magnetic carriers. Bio-separation is a crucial phenomenon for the success of several biological processes. Magnetic separation of cells or bio-molecules is more effectively done by adsorption/ desorption from the modiﬁed particles of spinel iron oxides. The synthesis parameters on the morphological and magnetic properties of spinel iron oxide are strongly dependent on the reaction conditions. A novel technology for DNA separation using the new magnetic materials can be promising for enhancing the efﬁciency of the bio-separation process. Classical methods for DNA/RNA isolation are either column-based techniques or include precipitation and centrifugation steps having the disadvantage of being time consuming, difﬁcult to automate or not useful for downscaling to small sample volumes . Effective cell separation is a primary and most important process for many clinical immunological applications using the magnetic oxide compounds. The selection of magnetic particles based on shape, size, and microstructures will signiﬁcantly affect the ﬁnal result of separation. Work presented here describes a new challenging process for efﬁcient and direct DNA separation with functionalized NiZn-ferrite ﬁbers. Magnetic separation is an emerging technology that uses magnetism for the efﬁcient separation of micrometer-sized
ARTICLE IN PRESS J.-H. Nam et al. / Journal of Magnetism and Magnetic Materials 321 (2009) 1389–1392
0 -20 60 -40
magnetic carriers from chemical or biological suspensions. Magnetic separation has many advantages compared to other techniques used for bio-separation or puriﬁcation and is generally done with iron oxide nanoparticles as magnetic carriers. Now, to make magnetic ceramic nanoﬁbers might be another way of gaining a large surface area and appropriate nanostructure for the application of DNA separation. The spinel ferrite MFe2O4 (M ¼ Ni, Zn) nanoﬁbers were synthesized by an electrospinnng process in this study. Raw materials used were iron (III) chloride (FeCl3), nickel acetate tetrahydrate (C4H6O4Ni . 4H2O) and zinc acetate dehydrate (C4H6O4Zn . 4H2O). The aqueous metal salt/polymer solution was prepared with polyvinyl pyrrolidone (PVP) in DMF (N,N-dimethylformamide) and metal salts under stirring at room temperature. The applied electric ﬁeld and spurting rate for spinning conditions were 10 kV, 2 ml/h, respectively. The obtained ﬁbers were calcined at 600 1C for 3 h and annealed at 900 1C in air. By tuning the viscosity of batch solution before electrospinning, we were able to control the microstructure of NiZn-ferrite ﬁber in the range 70–200 nm at 770 cp. The multiple individual grain size in a ferrite ﬁber was about 10–15 nm. The properties of those NiZn-ferrite ﬁbers as magnetic carrier were determined from X-ray diffraction, electron microscopy, thermal analysis, and magnetic measurement. The DNA adsorption efﬁciency yields compared to magnetite nanoparticle showed about 50% for UV-light wavelength, which can be modiﬁed and utilized for DNA separation with magnetic nanoﬁber in clinical applications. Prior to electrospinning, the viscosities of batch solutions were measured with the viscometer. The crystalline phases were idendiﬁed by X-ray diffraction (XRD); and the morphology of the NiZn-ferrite nanoﬁber were observed by FE-SEM. Reaction processes during the calcinations were studied by thermal analysis (TG–DTA) in the temperature range of 20–900 1C to determine calcination temperatures. Magnetic measurements were carried out at room temperature using VSM. Fig. 1 shows the results of microstructure of electrospun polymer and viscosity with polymer (PVP) content to optimize the experimental conditions of raw materials for fabrication of NiZnferrite ﬁber. The morphology and diameter of electrospun ﬁbers are dependent on a number of processing parameters that include the type of polymer in solution, the operational conditions of electrospinning unit . As shown in Fig. 1a–d, we can obtain the various electrospun PVP ﬁbers prepared with PVP content and the
40 -60 20
Temperature ( C) Fig. 2. Thermal analysis (TG–DTA) curves of metal salts/PVP solution.
: (Ni,Zn)Fe2O4 : FeOCl
2θ Fig. 3. XRD patterns of NiZn-ferrite (Ni0.4Zn0.6Fe2O4) nanoﬁbers fabricated at various ﬁring temperatures. (a) As electrospun, (b) calcined at 400 1C, (c) calcined at 600 1C, and (d) calcined at 600 1C and annealed at 900 1C, respectively.
1200 1000 800 600 400 200 0
Concentration of polymer (wt %)
Fig. 1. Various electrospinning conditions for PVP ﬁber made from (a) 5 wt% (27 cP), (b) 10% (180 cP), (c) 15% (770 cP), (d) 20% (1,515 cP) of the polymer, and (e) the viscosity at 2.3 cm1 shear rate increases with higher PVP concentration.
ARTICLE IN PRESS J.-H. Nam et al. / Journal of Magnetism and Magnetic Materials 321 (2009) 1389–1392
out of metal salts (Fe-chloride, Ni-acetate, Zn-acetate). An exothermic DTA peak at about 550 1C indicates the onset in crystallization of spinel structure of NiZn-ferrite ﬁber. The XRD patterns of NiZn-ferrite ﬁbers are presented in Fig. 3. The unreacted FeOCl phase appeared at 400 1C (Fig. 3b). NiZn-ferrite ﬁbers, thus, can be obtained at over 600 1C with single phase of spinel structure with good crystallinity. The molar ratio (Ni:Zn) of NiZn ferrite was selected as 0.4:0.6 (Ni0.4Zn0.6Fe2O4) due to its high saturation magnetization (Fig. 4). NiZn-ferrite ﬁbers obtained at various calcination temperatures show ferromagnetic behavior . It also appeared that the saturation magnetization (MS) of NiZn-ferrite nanoﬁber was dependent on the Ni/Zn molar ratio as is typically found in inverse spinel ferrites . The NiZn-ferrite (Ni0.4Zn0.6Fe2O4) ﬁbers fabricated by electrospinning process were also characterized by scanning electron microscope. Fig. 5 shows the microstructures of NiZn-ferrite (Ni0.4Zn0.6Fe2O4) nanoﬁbers calcined at various calcination temperatures. SEM images of NiZn-ferrite nanoﬁber in Fig. 5a–c shows the multiple grains as a polygonal grain growth with ﬁring temperature in matrix. The bubble-shaped individual grain in NiZn-ferrite ﬁber (Fig. 5a) was identiﬁed as an unreacted phase of FeOCl by EDS analysis (Fig. 5d). At 600 1C, no residual chloride of PVP was detected anymore (Fig. 5e) and pure NiZn-ferrite ﬁber obtained with a continuous structure. Magnetic separation is an emerging technology that uses magnetism for the efﬁcient separation of nano-sized paraand ferromagnetic particulate media from chemical or biological suspensions . The basic technology of using magnetic separation techniques to purify biological compounds (nucleic acids, proteins, etc.) and cells is interesting due to advantages over other techniques used for the same processes. The efﬁciency of magnetic separation is well suited for large-scale puriﬁcation using small particles of 0.05–0.1 mm in diameter. The increasing application of magnetic carriers in biochemical or molecular biology processing has many advantages compared to other nonmagnetic separation. Table 1 shows the variation of UV-light absorbance with adsorption time measured by UV/VIS spectrophotometer for characterization of DNA separation using NiZn-ferrite (Ni0.4Zn0.6Fe2O4)
ﬁber diameter. The formation of beads in electrospun ﬁbers in Fig. 1a and b can be affected by the solution properties as viscosity, surface tension, and the density of net charges carried by the liquid jet . It can be clearly presented that the viscosity of solution was dramatically increased at a proper concentration of polymer. The batch solution of sol precursor was affected the viscosity which was resulted in change of ferrite ﬁber diameter. The viscosity for high performance of ﬁber by electrospinning was obtained in the range 300–700 cP at a shear rate of 2.3 s1. In order to obtain a normal electrospun ﬁber (Fig. 1c and d), the PVP content should be over 15% in batch solution. Fig. 2 shows the characteristic thermal analysis (TGA and DTA) curves of the batch solution of metal salts with PVP. Between 200 and 300 1C, weight loss and an exothermic DTA peak in TGA were observed because of the decomposition of PVP which yields to an increasing viscosity. A further weight loss in TGA and exothermic DTA peaks at around 500–600 1C is consistent with the burning-
Saturation magnetization, MS (emu/g)
400 C o
50 40 30
4 3 2 1 0 0.2
Ni contents, x Fig. 4. Saturation magnetization (MS) of NixZn1xFe2O4 nanoﬁbers with Ni content at various ﬁring temperature.
2nd phase ( FeOCl)
c:\edax32\genesis\genmaps.spc 03-Apr-2008 13:57:40 LSecs : 44
c:\edax32\genesis\genmaps.spc 06-oct-2008 17:43:04 LSecs : 97 2.1
1.5 1.0 0.5
Zn Fe Ni
0.0 1.00 2.00 3.00 4.00 5.00 6.00 7.00 8.00 9.00 Energy - keV
1.00 2.00 3.00 4.00 5.00 6.00 7.00 8.00 9.00 10.0 Energy - keV
Fig. 5. SEM images of various NiZn-ferrite (Ni0.4Zn0.6Fe2O4) nanoﬁbers (a) calcined at 400 1C, (b) calcined at 600 1C, and (c) calcined at 600 1C and annealed at 900 1C. The EDS analysis peaks of some of the nanoﬁbers are shown in (d) calcined at 400 1C and (e) calcined at 600 1C.
ARTICLE IN PRESS 1392
J.-H. Nam et al. / Journal of Magnetism and Magnetic Materials 321 (2009) 1389–1392
Table 1 Characterization of DNA separation using NiZn ferrite (Ni0.4Zn0.6Fe2O4) nanoﬁbers. Adsorption time (h)
2 4 6
UV-light absorbance DNA only
NiZn ferrite ﬁber added
0.53 0.53 0.59
0.31 0.28 0.32
nanoﬁber. NiZn-ferrite ﬁbers thus clearly adsorb DNA, and NiZnferrite nanoﬁbers can be used like other magnetic carriers for DNA separation. Different incubation times do not produce signiﬁcantly different DNA adsorptions (Table 1). The magnetic ﬁber can also be suitable for the puriﬁcation with relatively high DNA adsorption efﬁciency, which can be modiﬁed and utilized for DNA separation with magnetic nanoﬁber as a novel material in clinical applications. The bio-compatibility of NiZn-ferrite nanoﬁber with a large surface area and the application to the DNA separation give promising experimental data for the further development of DNA puriﬁcation procedures. The fabrication of NiZn-ferrite nanoﬁber is presented as a preliminary work for new techniques of the magnetic separation, and further modiﬁcation will be undertaken
in a next step to make this method a successful DNA separation with functionalized magnetic nanoﬁbers that can be utilized in clinical diagnoses and biomolecular recognition. References  R. Ramaseshan, S. Sundarrajan, R. Jose, S. Ramakrishna, J. Appl. Phys. 102 (1999) 111101.  W. Sigmund, J. Yuh, H. Park, et al., J. Am. Ceram. Soc. 89 (2006) 395.  Y. Zhu, J.C. Zhang, J. Zhai, L. Jiang, Thin Solid Films 510 (2006) 271.  P.K. Panda, S. Ramakrishna, J. Mater. Sci. 42 (2007) 2189.  R.W. Tuttle, A. Chowdury, E.T. Bender, et al., Appl. Surface Sci. 254 (2008) 4925.  S.H. Xie, J.Y. Li, Y. Qiao, et al., Appl. Phys. Lett. 92 (2008) 062901.  A.K. Alves, F.A. Berutti, F.J. Clemens, et al., Mater. Res. Bull. 44 (2009) 312.  S. Madhugiri, W. Zhou, J.P. Ferraris, K.J. Balkus Jr., Microporous Mesoporous Mater. 63 (2003) 75.  H. Dai, J. Gong, H. Kim, D. Lee, Nanotechnology 13 (2002) 674.  D. Li, Y. Xia, Nano Lett. 3 (2003) 555.  A. Fenot, I.S. Chronakis, Curr. Opin. Colloid Interface Sci. 8 (2003) 64.  K.M. Sawicka, P. Gouma, J. Nanoparticle Res. 8 (2006) 769.  J. Oster, J. Parker, L. Brassard, J. Magn. Magn. Mater. 225 (2001) 145.  D. Li, Y. Xia, Adv. Mater. 14 (2004) 1151.  H. Fong, I. Chun, D.H. Reneker, Polymer 40 (1999) 4585.  D. Li, T. Herricks, Y. Xia, Appl. Phys. Lett. 83 (2003) 4586.  E.W. Gorter, Philips Res. Rep. 9 (1954), 295/321/403.  S. Berensmeier, Appl. Microbiol. Bioechnol. 73 (2006) 495.